#------------------------------------------------------------------------------
#$Date: 2016-02-21 02:03:34 +0200 (Sun, 21 Feb 2016) $
#$Revision: 176798 $
#$URL: svn://www.crystallography.net/cod/cif/2/23/60/2236087.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2236087
loop_
_publ_author_name
'Artner, Christine'
'Weil, Matthias'
_publ_section_title
;
 Pb₆Co₉(TeO₆)₅
;
_journal_coeditor_code           BR2208
_journal_issue                   9
_journal_name_full               'Acta Crystallographica Section E'
_journal_page_first              i71
_journal_paper_doi               10.1107/S1600536812037038
_journal_volume                  68
_journal_year                    2012
_chemical_formula_iupac          'Pb6 Co9 (Te O6)5'
_chemical_formula_structural     'Pb6 Co9 (Te O6)5'
_chemical_formula_sum            'Co9 O30 Pb6 Te5'
_chemical_formula_weight         2891.51
_chemical_name_systematic
;
hexalead(II) nonacobalt(II) pentatellurate(VI)
;
_space_group_IT_number           182
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  'P 6c 2c'
_symmetry_space_group_name_H-M   'P 63 2 2'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            2
_cell_length_a                   10.39150(10)
_cell_length_b                   10.39150(10)
_cell_length_c                   13.6273(2)
_cell_measurement_reflns_used    6739
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      36.766
_cell_measurement_theta_min      2.751
_cell_volume                     1274.37(3)
_computing_cell_refinement       'SAINT (Bruker, 2004)'
_computing_data_collection       'APEX2 (Bruker, 2004)'
_computing_data_reduction        'SAINT (Bruker, 2004)'
_computing_molecular_graphics    'ATOMS for Windows (Dowty, 2006)'
_computing_publication_material  'publCIF (Westrip, 2010)'
_computing_structure_refinement  'SHELXL97 (Sheldrick, 2008)'
_computing_structure_solution    'SHELXS97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measurement_device_type  'Bruker APEXII CCD'
_diffrn_measurement_method       'ω and φ scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0680
_diffrn_reflns_av_sigmaI/netI    0.0320
_diffrn_reflns_limit_h_max       17
_diffrn_reflns_limit_h_min       -16
_diffrn_reflns_limit_k_max       17
_diffrn_reflns_limit_k_min       -17
_diffrn_reflns_limit_l_max       23
_diffrn_reflns_limit_l_min       -22
_diffrn_reflns_number            45686
_diffrn_reflns_theta_full        37.57
_diffrn_reflns_theta_max         37.57
_diffrn_reflns_theta_min         2.26
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    50.890
_exptl_absorpt_correction_T_max  0.2002
_exptl_absorpt_correction_T_min  0.1231
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details
;
(HABITUS; Herrendorf, 1997)
;
_exptl_crystal_colour            'dark red'
_exptl_crystal_density_diffrn    7.535
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       parallelepiped
_exptl_crystal_F_000             2470
_exptl_crystal_size_max          0.072
_exptl_crystal_size_mid          0.060
_exptl_crystal_size_min          0.048
_refine_diff_density_max         2.958
_refine_diff_density_min         -2.587
_refine_ls_abs_structure_details 'Flack (1983), 882 Friedel pairs'
_refine_ls_abs_structure_Flack   0.134(10)
_refine_ls_extinction_coef       0.00019(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     'SHELXL97 (Sheldrick, 2008)'
_refine_ls_goodness_of_fit_ref   1.090
_refine_ls_matrix_type           full
_refine_ls_number_parameters     81
_refine_ls_number_reflns         2262
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.090
_refine_ls_R_factor_all          0.0335
_refine_ls_R_factor_gt           0.0246
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0244P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0545
_refine_ls_wR_factor_ref         0.0559
_reflns_number_gt                1908
_reflns_number_total             2262
_reflns_threshold_expression     I>2σ(I)
_cod_data_source_file            br2208.cif
_cod_data_source_block           I
_cod_database_code               2236087
_cod_database_fobs_code          2236087
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'x-y, x, z+1/2'
'-y, x-y, z'
'-x, -y, z+1/2'
'-x+y, -x, z'
'y, -x+y, z+1/2'
'-y, -x, -z+1/2'
'x-y, -y, -z'
'x, x-y, -z+1/2'
'y, x, -z'
'-x+y, y, -z+1/2'
'-x, -x+y, -z'
loop_
_atom_site_type_symbol
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_occupancy
_atom_site_symmetry_multiplicity
Pb Pb1 0.26736(3) 0.26736(3) 0.0000 0.01216(6) Uani d S 1 2
Pb Pb2 0.38848(3) 1.0000 0.0000 0.01881(8) Uani d S 1 2
Te Te1 0.3333 0.6667 -0.09611(4) 0.00407(10) Uani d S 1 3
Te Te2 0.16730(4) 0.33460(9) 0.2500 0.00433(8) Uani d S 1 2
Co Co1 0.3333 0.6667 0.11832(9) 0.0066(2) Uani d S 1 3
Co Co2 0.16885(10) 0.3377(2) -0.2500 0.00664(18) Uani d S 1 2
Co Co3 0.0000 0.0000 0.2500 0.0087(3) Uani d S 1 6
Co Co4 0.00992(19) 0.50496(10) -0.2500 0.00566(18) Uani d S 1 2
O O1 0.3366(5) 0.3241(5) -0.1717(3) 0.0077(8) Uani d . 1 1
O O2 0.1726(7) 0.5050(6) -0.1628(3) 0.0083(10) Uani d . 1 1
O O3 0.1702(7) 0.1801(6) 0.3277(3) 0.0105(9) Uani d . 1 1
O O5 0.3239(8) 0.4818(6) 0.3295(3) 0.0076(10) Uani d . 1 1
O O6 0.3481(4) 0.5265(4) -0.0034(4) 0.0069(6) Uani d . 1 1
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Pb Pb -3.3944 10.1111 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Te Te -0.5308 1.6751 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle
O6 Pb1 O6 10 . 84.58(16)
O6 Pb1 O1 10 10 79.26(18)
O6 Pb1 O1 . 10 77.79(18)
O6 Pb1 O1 10 . 77.79(18)
O6 Pb1 O1 . . 79.26(18)
O1 Pb1 O1 10 . 148.79(19)
O6 Pb1 O3 10 6_554 95.87(13)
O6 Pb1 O3 . 6_554 133.98(17)
O1 Pb1 O3 10 6_554 147.68(15)
O1 Pb1 O3 . 6_554 56.26(15)
O6 Pb1 O3 10 11 133.98(17)
O6 Pb1 O3 . 11 95.87(13)
O1 Pb1 O3 10 11 56.26(15)
O1 Pb1 O3 . 11 147.68(15)
O3 Pb1 O3 6_554 11 114.8(2)
O6 Pb1 O3 10 2_554 138.20(17)
O6 Pb1 O3 . 2_554 95.05(13)
O1 Pb1 O3 10 2_554 141.63(15)
O1 Pb1 O3 . 2_554 61.26(14)
O3 Pb1 O3 6_554 2_554 55.44(13)
O3 Pb1 O3 11 2_554 87.73(10)
O6 Pb1 O3 10 9 95.05(13)
O6 Pb1 O3 . 9 138.20(17)
O1 Pb1 O3 10 9 61.26(14)
O1 Pb1 O3 . 9 141.63(15)
O3 Pb1 O3 6_554 9 87.73(10)
O3 Pb1 O3 11 9 55.44(13)
O3 Pb1 O3 2_554 9 111.4(2)
O6 Pb2 O6 12_665 3_665 83.17(17)
O6 Pb2 O2 12_665 10_565 61.34(16)
O6 Pb2 O2 3_665 10_565 107.91(19)
O6 Pb2 O2 12_665 5_565 107.91(19)
O6 Pb2 O2 3_665 5_565 61.34(16)
O2 Pb2 O2 10_565 5_565 166.8(3)
O6 Pb2 O5 12_665 9_565 106.77(19)
O6 Pb2 O5 3_665 9_565 68.25(16)
O2 Pb2 O5 10_565 9_565 66.27(12)
O2 Pb2 O5 5_565 9_565 112.94(13)
O6 Pb2 O5 12_665 6_564 68.25(16)
O6 Pb2 O5 3_665 6_564 106.77(19)
O2 Pb2 O5 10_565 6_564 112.94(13)
O2 Pb2 O5 5_565 6_564 66.27(12)
O5 Pb2 O5 9_565 6_564 173.7(3)
O6 Pb2 O6 12_665 5_565 138.39(2)
O6 Pb2 O6 3_665 5_565 55.23(15)
O2 Pb2 O6 10_565 5_565 126.25(15)
O2 Pb2 O6 5_565 5_565 55.67(17)
O5 Pb2 O6 9_565 5_565 60.10(16)
O5 Pb2 O6 6_564 5_565 120.76(15)
O6 Pb2 O6 12_665 10_565 55.23(15)
O6 Pb2 O6 3_665 10_565 138.39(2)
O2 Pb2 O6 10_565 10_565 55.67(17)
O2 Pb2 O6 5_565 10_565 126.25(15)
O5 Pb2 O6 9_565 10_565 120.76(15)
O5 Pb2 O6 6_564 10_565 60.10(16)
O6 Pb2 O6 5_565 10_565 166.38(13)
O6 Pb2 O3 12_665 6_564 120.59(18)
O6 Pb2 O3 3_665 6_564 121.18(18)
O2 Pb2 O3 10_565 6_564 130.9(2)
O2 Pb2 O3 5_565 6_564 60.21(13)
O5 Pb2 O3 9_565 6_564 132.1(2)
O5 Pb2 O3 6_564 6_564 53.44(14)
O6 Pb2 O3 5_565 6_564 86.29(19)
O6 Pb2 O3 10_565 6_564 84.37(18)
O6 Pb2 O3 12_665 9_565 121.18(18)
O6 Pb2 O3 3_665 9_565 120.59(18)
O2 Pb2 O3 10_565 9_565 60.21(13)
O2 Pb2 O3 5_565 9_565 130.9(2)
O5 Pb2 O3 9_565 9_565 53.44(14)
O5 Pb2 O3 6_564 9_565 132.1(2)
O6 Pb2 O3 5_565 9_565 84.37(18)
O6 Pb2 O3 10_565 9_565 86.29(19)
O3 Pb2 O3 6_564 9_565 93.32(14)
O2 Te1 O2 5_565 . 99.15(18)
O2 Te1 O2 5_565 3_665 99.15(18)
O2 Te1 O2 . 3_665 99.15(18)
O2 Te1 O6 5_565 5_565 90.7(2)
O2 Te1 O6 . 5_565 85.2(2)
O2 Te1 O6 3_665 5_565 168.4(2)
O2 Te1 O6 5_565 3_665 85.2(2)
O2 Te1 O6 . 3_665 168.4(2)
O2 Te1 O6 3_665 3_665 90.7(2)
O6 Te1 O6 5_565 3_665 84.0(2)
O2 Te1 O6 5_565 . 168.4(2)
O2 Te1 O6 . . 90.7(2)
O2 Te1 O6 3_665 . 85.2(2)
O6 Te1 O6 5_565 . 84.0(2)
O6 Te1 O6 3_665 . 84.0(2)
O5 Te2 O5 . 11 92.5(3)
O5 Te2 O3 . 11 177.8(2)
O5 Te2 O3 11 11 89.6(2)
O5 Te2 O3 . . 89.6(2)
O5 Te2 O3 11 . 177.8(2)
O3 Te2 O3 11 . 88.2(2)
O5 Te2 O1 . 2 93.3(2)
O5 Te2 O1 11 2 85.9(2)
O3 Te2 O1 11 2 87.0(2)
O3 Te2 O1 . 2 93.7(2)
O5 Te2 O1 . 10 85.9(2)
O5 Te2 O1 11 10 93.3(2)
O3 Te2 O1 11 10 93.7(2)
O3 Te2 O1 . 10 87.0(2)
O1 Te2 O1 2 10 179.0(3)
O5 Co1 O5 9_565 11 108.14(14)
O5 Co1 O5 9_565 7_665 108.14(14)
O5 Co1 O5 11 7_665 108.14(14)
O5 Co1 O6 9_565 5_565 87.99(18)
O5 Co1 O6 11 5_565 85.39(19)
O5 Co1 O6 7_665 5_565 153.55(18)
O5 Co1 O6 9_565 3_665 85.39(19)
O5 Co1 O6 11 3_665 153.55(18)
O5 Co1 O6 7_665 3_665 87.99(18)
O6 Co1 O6 5_565 3_665 72.17(17)
O5 Co1 O6 9_565 . 153.55(18)
O5 Co1 O6 11 . 87.99(18)
O5 Co1 O6 7_665 . 85.39(18)
O6 Co1 O6 5_565 . 72.17(17)
O6 Co1 O6 3_665 . 72.17(17)
O2 Co2 O2 11_554 . 87.8(3)
O2 Co2 O3 11_554 10 92.52(17)
O2 Co2 O3 . 10 174.4(3)
O2 Co2 O3 11_554 2_554 174.4(3)
O2 Co2 O3 . 2_554 92.52(17)
O3 Co2 O3 10 2_554 87.7(2)
O2 Co2 O1 11_554 . 89.3(2)
O2 Co2 O1 . . 95.5(2)
O3 Co2 O1 10 . 78.9(2)
O3 Co2 O1 2_554 . 96.2(2)
O2 Co2 O1 11_554 11_554 95.5(2)
O2 Co2 O1 . 11_554 89.3(2)
O3 Co2 O1 10 11_554 96.2(2)
O3 Co2 O1 2_554 11_554 78.9(2)
O1 Co2 O1 . 11_554 173.3(3)
O3 Co3 O3 7 . 175.2(5)
O3 Co3 O3 7 3 79.5(4)
O3 Co3 O3 . 3 96.96(14)
O3 Co3 O3 7 5 86.8(4)
O3 Co3 O3 . 5 96.96(14)
O3 Co3 O3 3 5 96.96(14)
O3 Co3 O3 7 11 96.96(14)
O3 Co3 O3 . 11 79.5(4)
O3 Co3 O3 3 11 86.8(4)
O3 Co3 O3 5 11 175.2(5)
O3 Co3 O3 7 9 96.96(14)
O3 Co3 O3 . 9 86.8(4)
O3 Co3 O3 3 9 175.2(5)
O3 Co3 O3 5 9 79.5(4)
O3 Co3 O3 11 9 96.96(14)
O2 Co4 O2 . 9_564 89.8(3)
O2 Co4 O1 . 5_565 96.9(2)
O2 Co4 O1 9_564 5_565 91.0(2)
O2 Co4 O1 . 11_554 91.0(2)
O2 Co4 O1 9_564 11_554 96.9(2)
O1 Co4 O1 5_565 11_554 168.8(4)
O2 Co4 O5 . 8_565 174.7(3)
O2 Co4 O5 9_564 8_565 90.92(16)
O1 Co4 O5 5_565 8_565 77.8(2)
O1 Co4 O5 11_554 8_565 94.2(2)
O2 Co4 O5 . 2_554 90.92(16)
O2 Co4 O5 9_564 2_554 174.7(3)
O1 Co4 O5 5_565 2_554 94.2(2)
O1 Co4 O5 11_554 2_554 77.8(2)
O5 Co4 O5 8_565 2_554 88.9(3)
Te2 O1 Co4 6_554 3_665 98.54(19)
Te2 O1 Co2 6_554 . 96.67(17)
Co4 O1 Co2 3_665 . 89.3(2)
Te2 O1 Pb1 6_554 . 116.6(2)
Co4 O1 Pb1 3_665 . 136.07(18)
Co2 O1 Pb1 . . 110.4(2)
Te1 O2 Co4 . . 129.1(3)
Te1 O2 Co2 . . 130.4(4)
Co4 O2 Co2 . . 89.87(19)
Te1 O2 Pb2 . 3_665 95.48(17)
Co4 O2 Pb2 . 3_665 96.4(2)
Co2 O2 Pb2 . 3_665 111.0(2)
Te2 O3 Co2 . 6 97.34(17)
Te2 O3 Co3 . . 96.2(2)
Co2 O3 Co3 6 . 92.8(3)
Te2 O5 Co1 . 7_665 125.5(4)
Te2 O5 Co4 . 6 97.7(2)
Co1 O5 Co4 7_665 6 120.3(3)
Te2 O5 Pb2 . 2_655 117.3(2)
Co1 O5 Pb2 7_665 2_655 97.82(18)
Co4 O5 Pb2 6 2_655 95.2(2)
Te1 O6 Co1 . . 86.54(14)
Te1 O6 Pb1 . . 136.5(2)
Co1 O6 Pb1 . . 127.8(2)
Te1 O6 Pb2 . 5_565 103.41(16)
Co1 O6 Pb2 . 5_565 100.34(16)
Pb1 O6 Pb2 . 5_565 96.12(13)
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
Pb1 O6 10 2.387(4) ?
Pb1 O6 . 2.387(4) ?
Pb1 O1 10 2.432(4) ?
Pb1 O1 . 2.432(4) ?
Pb1 O3 6_554 3.327(7) ?
Pb1 O3 11 3.327(7) ?
Pb1 O3 2_554 3.453(7) ?
Pb1 O3 9 3.453(7) ?
Pb1 Pb2 5_565 3.5764(4) ?
Pb1 Pb2 3_665 3.5777(2) ?
Pb2 O6 12_665 2.420(3) ?
Pb2 O6 3_665 2.420(3) ?
Pb2 O2 10_565 2.726(5) ?
Pb2 O2 5_565 2.726(5) ?
Pb2 O5 9_565 2.727(5) ?
Pb2 O5 6_564 2.727(5) ?
Pb2 O6 5_565 3.155(3) ?
Pb2 O6 10_565 3.155(3) ?
Pb2 O3 6_564 3.230(4) ?
Pb2 O3 9_565 3.230(4) ?
Te1 O2 5_565 1.906(5) ?
Te1 O2 . 1.906(5) y
Te1 O2 3_665 1.906(5) ?
Te1 O6 5_565 1.991(4) ?
Te1 O6 3_665 1.991(4) ?
Te1 O6 . 1.991(4) y
Te2 O5 . 1.917(6) y
Te2 O5 11 1.917(6) ?
Te2 O3 11 1.937(7) ?
Te2 O3 . 1.937(7) y
Te2 O1 2 1.939(5) y
Te2 O1 10 1.939(5) ?
Co1 O5 9_565 2.004(6) ?
Co1 O5 11 2.004(6) y
Co1 O5 7_665 2.004(6) ?
Co1 O6 5_565 2.262(5) ?
Co1 O6 3_665 2.262(5) ?
Co1 O6 . 2.262(5) y
Co2 O2 11_554 2.090(6) ?
Co2 O2 . 2.090(6) y
Co2 O3 10 2.090(8) y
Co2 O3 2_554 2.090(8) ?
Co2 O1 . 2.108(6) y
Co2 O1 11_554 2.108(6) ?
Co3 O3 7 2.107(4) ?
Co3 O3 . 2.107(4) y
Co3 O3 3 2.107(4) ?
Co3 O3 5 2.107(4) ?
Co3 O3 11 2.107(4) ?
Co3 O3 9 2.107(4) ?
Co4 O2 . 2.067(7) y
Co4 O2 9_564 2.067(7) ?
Co4 O1 5_565 2.071(4) y
Co4 O1 11_554 2.071(4) ?
Co4 O5 8_565 2.116(7) y
Co4 O5 2_554 2.116(7) ?
